Pipe ProcessesUNIT: 1 UNIT: 1
In cooperation with subject matter expert:
In cooperation with subject matter expert:
© SOLAS 2014
Table of Contents
Unit Objective ... 1
Learning Outcome ... 2
1.0 Introduction to Pipe and Tube ... 3
1.1 Pipe and Tube ... 3
1.2 Difference Between Pipe and Tube ... 3
1.3 Markings on Pipe and Tube ... 4
2.0 Manufacture of Pipe and Tube ... 5
2.1 How Pipe and Tube are Made ... 5
2.2 Finishing Processes for Pipe and Tube ... 5
2.3 Non Destructive Tests for Pipe and Tube ... 7
3.0 Materials Used for Pipe and Tube ... 8
3.1 Different Materials Used for Pipe and Tube ... 8
3.2 Concrete and Ceramic Pipes ... 8
3.3 Plastic Pipes ... 8
3.4 Metal Pipes and Tubes ... 9
3.5 Stainless Steel Pipes and Tubes ... 9
3.6 Material Traceability ... 10
4.0 Classification of Pipes Sizes ... 11
4.1 Introduction to Pipe Sizes ... 11
4.2 Nominal Pipe Size and Nominal Diameter Pipe Size ... 11
4.3 International Standards for Pipe Sizes ... 12
4.4 Pipe Sizes for Other Materials ... 12
4.5 Sizes for Copper Tube ... 13
4.6 Sizes for Stainless Steel Tube ... 14
5.0 Pressure Ratings for Pipes and Tubes ... 16
5.1 Pressure Ratings for Pipe and Tube ... 16
5.2 Wall Thickness Calculations for Straight Pipe Under Internal Pressure ... 17
6.0 Physical Properties of Piping Materials ... 21
6.1 Physical Properties of Piping Materials ... 21
Exercises ... 23
There are seven Units in Module 3 for Pipe Processes. Unit 1 focuses on Piping Materials, Unit 2; Piping components and fittings, Unit 3; Bill of Materials, Unit 4; Pipe Preparation, Unit 5; Pipe Joining, Unit 6; Pipe threading and testing and Unit 7 Pipe bending.
In this unit you will be introduced to the different Piping materials available to the pipefitting industry, their properties, how they are classified and why they are selected for different applications and services.
Module 3 Pipe Processes Unit 1 Pipe Materials Unit 2 Piping Component and Fittings Unit 3 Bill of Materials Unit 4 Pipe Preparation Unit 5 Pipe Joining Unit 6 Pipe Threading and Testing Unit 7 Pipe Bending
By the end of this unit each apprentice will be able to:
List and describe the different materials used in the pipe industry List and describe how pipes are classified in according with wall
thickness, method of manufacture and grades of material.
Describe pressure ratings of different pipe schedules and grades of
Differentiate between pipe and tube and how their diameters are
Recognise the most commonly used pipe sizes and the standard lengths
supplied by manufacturers
Define some of the physical properties in relation to piping materials Identify a selection of alloyed non-ferrous based pipes and explain why
they are used for certain applications
List and describe types and materials used for plastic pipe in the pipe
industry and state their uses
List and describe the types of tube and tubing used in the pipe trades
1.0 Introduction to Pipe and Tube
1.1 Pipe and Tube
A pipe is round tubular section or hollow cylinder used mainly to convey media. It may also be used for structural applications; however in this instance we will concentrate on its use in the process industry. Pipe is generally
manufactured to several long-standing and broadly applicable industrial standards. While similar standards exist for specific industry application tubing, tube is often made to custom sizes and a broader range of diameters and tolerances. Many industrial and government standards exist for the production of pipe and tubing. The term "tube" is also commonly applied to non-cylindrical sections (i.e. square or rectangular tubing).
1.2 Difference Between Pipe and Tube
In general terms the appellations pipe and tube are almost interchangeable, but in the pipe fitting industry and engineering discipline the terms are uniquely defined.
Depending on the applicable standard to which it is manufactured, pipe is specified by the internal diameter (ID) and a wall thickness, the inside diameter called the nominal diameter may not exactly match the pipe size as it varies with the wall thickness. For example the ID of an 8” pipe varies from
213.54mm ID for Sch5 pipe to 193.68mm for Sch40 pipe.
Tube is most often defined by the outside diameter (OD) and a wall thickness. Therefore 8” tube would have an outside diameter of 203.2mm.
Key Learning Points
Introduction to pipe and tube
Identify the differences between pipe and tube Identify the common markings for pipe and tube
1.3 Markings on Pipe and Tube
As there are many different types of pipe and tube and different standards that are applicable for each, it is not possible to give a definitive list of the exact information required to be marked on pipe and tube; however the common requirements would be as follows and should be continuously marked down its whole length:
Nominal Pipe Size (Nominal Bore) Schedule (Wall Thickness)
Method of Manufacture (Seamless or Welded) Heat Number
2.0 Manufacture of Pipe and Tube
2.1 How Pipe and Tube are Made
There are two main processes for metallic pipe manufacture. Seamless (SMLS) pipe is formed by drawing a solid billet over a piercing rod to create the hollow shell. Seamless pipe is generally more expensive to manufacture but provides higher pressure ratings. Welded pipe is formed by rolling plate and welding the seam. The weld seam is formed by Electric Resistance Welded (ERW) or Electric Fusion Welded (EFW) and is usually ground flush with the parent material as part of the manufacturing process. The weld zone can also be heat treated, so the seam is less visible. Welded pipe often has tighter dimensional tolerances than seamless, and can be cheaper if manufactured in large quantities. Large diameter pipe (about 10” or greater) may be ERW, or Submerged Arc Welded (SAW) pipe. Metal tubing due to the thinner wall thickness can be extruded but not always and many sanitary tubes such as hygienic stainless steel has a welded seam. Plastics are generally extruded due to the ease of handling the base materials. The illustration below shows the different ways that pipe are manufactured:
2.2 Finishing Processes for Pipe and Tube
There are limitations to the hot manufacturing processes for pipe and tube such as:
Small diameters are impracticable Thin walls are difficult to obtain Tolerances are difficult to control
Mechanical properties cannot be controlled adequately The surface finish on both the OD and the ID are rough Sophisticated shapes are not possible
For these reasons pipe and tube are cold worked after extrusion or seam welding.
Key Learning Points
Describe the basic methods of how pipe and tube are made Identify the finishing process that pipe and tube undergo Identify the type of non destructive testing that pipe and tube
2.3 Non Destructive Tests for Pipe and Tube
Non-destructive tests do not damage the pipe or tube being tested and so they are frequently incorporated into the end of the production line. The following give a brief explanation of the common types of NDT available:
This test involves ultrasonic sound waves being aimed, via a coupling medium, at the material to be tested. A proportion is bounced back at the interface but the remainder enter the material and bounce from the internal surface, to the external surface, where a transducer converts them into electrical energy. This is then monitored on a cathode ray tube where results are compared with those from a calibration standard. Any deviations from the standard are visible, thus indicating cracks or internal defects.
This involves inducing eddy currents into the material by exciting a coil which surmounts two narrow search coils surrounding the material. Any discontinuities in material are found by comparing the electrical conditions that exist in the two search coils. The fault signals are amplified and can be shown on a cathode ray tube or as an audible signal.
This is used to test the manufactured items under a pressure equivalent to or greater than pressure to be encountered in service. It involves filling the tube with water, which cannot be compressed, and increasing the pressure inside the
tube to that specified.
Magnetic Particle Testing
This method of testing is used when trying to detect discontinuities in material of ferromagnetic structure. The method is based on the principle that an imperfection will cause a distortion in the magnetic field pattern of a magnetised component. The imperfection can be revealed by applying magnetic particles to the component during or after magnetisation.
Radiographic (X-Ray) Testing
This is usually used to determine whether a weld is sound. It involves subjecting a weld or weld area to an X-Ray source with an X-Ray sensitive film plate on the under side of the weld. The results are shown on the developed film (a photomicrograph) and interpreted according to specification.
This is used to detect cracks and involves spraying a dye on the area to be tested. After allowing time for penetration the surplus dye is removed and the area is then sprayed with a white developer. Any faults are revealed as coloured lines or spots caused by the developer absorbing the dye seeping from the cracks. If more sensitive results are required, a fluorescent dye is used and the same process is followed. When viewed under ultraviolet light any defects show as a highly fluorescent line or spot.
3.0 Materials Used for Pipe and Tube
3.1 Different Materials Used for Pipe and Tube
Pipe may be made from a variety of materials. In the past, materials have included wood and lead (Latin for lead is plumbum, from which we get the word plumbing). Nowadays the manufacturing of pipe uses many different
materials including ceramics, fiberglass, concrete, plastics and metals.
Concrete and ceramic Plastic
special piping materials such as glass or lined pipe
3.2 Concrete and Ceramic Pipes
Pipes may be made from concrete or ceramic materials. These pipes are usually used for low pressure applications such as gravity flow or drainage underground. Concrete pipes usually have a receiving bell or a stepped fitting, with various sealing methods applied at installation. Ceramic pipes are used for underground drainage which may be exposed to corrosive chemicals. These types of pipes are relatively inexpensive for the diameters in question and allow for ease of installation in rough site conditions.
3.3 Plastic Pipes
Plastic tubing is widely used for its light weight, chemical resistance, non-corrosive properties, and ease of making connections. Plastic materials include polyvinyl chloride (PVC), chlorinated polyvinyl chloride (CPVC), fibre reinforced plastic (FRP), reinforced polymer mortar (RPMP), polypropylene (PP), polyethylene (PE), cross-linked high-density polyethylene (PEX), polybutylene (PB), and acrylonitrile butadiene styrene (ABS), for example.
Key Learning Points
Identify common materials used for pipe and tube Identify why different materials are used
Identify the different properties of materials used for pipe and tube Identify different uses for the different materials
3.4 Metal Pipes and Tubes
Metallic pipes are commonly made from steel or iron; the metal chemistry and its finish are peculiar to the use fit and form. Typically metallic piping may be made of steel or iron, such as unfinished, black (lacquer) steel, carbon steel, stainless steel or galvanized steel, brass, and ductile iron. Aluminium pipe or tubing may be utilized where iron is incompatible with the service fluid or where weight is a concern; aluminium is also used for heat transfer tubing such
as in refrigerant systems. Copper tubing is popular for domestic water (potable) plumbing systems; copper may be used where heat transfer is desirable (i.e. radiators or heat exchangers). Inconel, chrome moly, and titanium steel alloys are used for high temperature and pressure piping in process systems where corrosion resistance is important.
3.5 Stainless Steel Pipes and Tubes
Stainless steel pipe and tubing are used for a variety of reasons: to resist corrosion and oxidation, to resist high temperatures, for cleanliness and low maintenance costs, and to maintain the purity of materials which come In contact with stainless. There are more than 60 grades of stainless steel available. The ability of stainless steel to resist corrosion is achieved by the addition of a minimum of 12% chromium to the iron alloy. Additions of other elements affect other properties. The inherent characteristics of stainless steel permit the design of thin wall piping systems without fear of early failure due to corrosion. Because of the thinner wall thickness of stainless steel tube it is not possible to thread tube therefore this was overcome by fusion welding to join such pipe and tubing.
Type 304 stainless is the most widely used analysis for general corrosive resistant tubing and pipe applications, it is used in chemical plants, refineries, paper mills, and food processing industries. Type 304 has a maximum carbon content of .08%. It is not recommended for use in the temperature range between 400°C and 900°C due to carbide precipitation at the grain boundaries which can result in inter-granular corrosion and early failure under certain
Type 304L. Is the same as 304 except that a 0.03% maximum carbon content is maintained which precludes carbon precipitation and permits the use of this analysis in welded assemblies under more severe corrosive conditions. Type 318 is much more resistant to pitting than other chromium nickel alloys due to the addition of 2% to 3% molybdenum. it is particularly valuable wherever acids, brines, sulphur water, seawater or halogen salts are encountered. Type 316 is widely used in the sulphite paper industry and for manufacturing chemical plant apparatus, photographic equipment, and plastics. Type 316L, like 304L, is held to a maximum carbon content of .03%. This permits its use in welded assemblies without the need of final heat treatment. It is used extensively for pipe assemblies with welded fitting.
3.6 Material Traceability
Manufacturing standards for pipes commonly require a test of chemical composition and a series of mechanical strength tests for each heat of pipe. A heat of pipe is all forged from the same cast ingot, and therefore had the same chemical composition. Mechanical tests may be associated to a lot of pipe, which would be all from the same heat and have been through the same heat treatment processes. The manufacturer performs these tests and reports the composition in a mill traceability report and the mechanical tests in a material test report, both of which are referred to by the acronym MTR. Material with these associated test reports is called traceable. For critical applications, third party verification of these tests may be required; in this case an independent lab will produce a certified material test report (CMTR), and the material will be called certified. By etching the heat number on the components made from this batch of material, it ensures that there is full traceability from the component to the material certificate and therefore the chemical composition of the component is known.
Maintaining the traceability between the material and this paperwork is an important quality assurance issue. QA often requires the heat number to be written on the pipe. Precautions must also be taken to prevent the introduction of counterfeit materials. As a back up to etching/labelling of the material identification on the pipe, Positive Material Identification (PMI) is performed using a handheld device; the device scans the pipe material using an emitted electromagnetic wave (x-ray fluorescence/XRF) and receives a reply that is spectrographically analysed.
4.0 Classification of Pipes Sizes
4.1 Introduction to Pipe Sizes
Pipe sizes can be confusing because the terminology may relate to historical dimensions. For example, a half-inch iron pipe doesn't have any dimension that is a half inch. Initially, a half inch pipe did have an internal dimension of 0.5” but it also had thick walls. As technology improved, the wall thickness got thinner (saving material costs), but the outside diameter stayed the same so it could mate with existing older pipe. The history of copper pipe is similar. In the 1930s, the pipe was designated by its internal diameter and a 1/16” wall thickness. Consequently, a 1” copper pipe would have a 1 1/8” outside diameter. The outside diameter was the important dimension for mating with fittings. The wall thickness on modern copper is usually thinner than 1/16”, so the internal diameter is only "nominal" rather than a controlling dimension. Newer pipe technologies sometimes adopted a sizing system as it’s own. PVC pipe uses the nominal pipe size.
4.2 Nominal Pipe Size and Nominal Diameter
Nominal Pipe Size (NPS) is a North American set of standard sizes for pipes used for high or low pressures and temperatures. Pipe size is specified with two non-dimensional numbers: a nominal pipe size (NPS) based on inches, and a schedule (Sch.) which specifies the wall thickness. The European designation equivalent to NPS is DN (Diamètre Nominal/nominal diameter), in which sizes are measured in millimetres. The term NB (nominal bore) is also frequently used interchangeably with NPS. Designating the outside diameter allows pipes of the same size to be fit together no matter what the wall thickness.
Pipe sizes are documented by many different international standards, including some of the following:
DIN EN 10217-7 / DIN EN 10216-5
BS EN 10255 in the United Kingdom and Europe. API Range Eg: API 5L Grade B
ASME SA106 Grade B (Seamless carbon steel pipe for high
ASTM A312 (Seamless and welded austenitic stainless steel pipe) ASTM C76 (Concrete Pipe)
Key Learning Points
Identify different specifications Customer specifications
4.3 International Standards for Pipe Sizes
For pipe sizes less than DN 350 (NPS 14”), both methods give a
nominal value for the OD that is rounded off and is not the same as the actual OD. For example, NPS 2” and DN 50 are the same pipe, but the actual OD is 2.375”, or 60.325mm. The only way to obtain the actual OD is to look it up in a reference table.
For pipe sizes of DN 350 (NPS 14”) and greater the NPS size is the
actual diameter in inches and the DN size is equal to NPS times 25 rounded to a convenient multiple of 50. For example, NPS 14” has an OD of 14”, or 355.6mm, and is equivalent to DN 350.
Since the outside diameter is fixed for a given pipe size, the inside diameter will vary depending on the wall thickness of the pipe. For example, 2" Schedule 80 (or Sch 80) pipe has thicker walls and therefore a smaller inside diameter than 2" Schedule 40 pipe. The table below lists the dimensions for 1/8” to 3” Pipe in both inches and millimetres and gives the different wall thicknesses for the different schedules. NPS Inches DN mm OD Inches (millimetres)
Wall Thickness - inches (millimetres) SCH 5 SCH 10 SCH 40 SCH 80 ⅛ 6 0.405 in (10.29 mm) 0.035 in (0.889 mm) 0.049 in (1.245 mm) 0.068 in (1.727 mm) 0.095 in (2.413 mm) ¼ 8 0.540 in (13.72 mm) 0.049 in (1.245 mm) 0.065 in (1.651 mm) 0.088 in (2.235 mm) 0.119 in (3.023 mm) ⅜ 10 0.675 in (17.15 mm) 0.049 in (1.245 mm) 0.065 in (1.651 mm) 0.091 in (2.311 mm) 0.126 in (3.200 mm) ½ 15 0.840 in (21.34 mm) 0.065 in (1.651 mm) 0.083 in (2.108 mm) 0.109 in (2.769 mm) 0.147 in (3.734 mm) ¾ 20 1.050 in (26.67 mm) 0.065 in (1.651 mm) 0.083 in (2.108 mm) 0.113 in (2.870 mm) 0.154 in (3.912 mm) 1 25 1.315 in (33.40 mm) 0.065 in (1.651 mm) 0.109 in (2.769 mm) 0.133 in (3.378 mm) 0.179 in (4.547 mm) 1¼ 32 1.660 in (42.16 mm) 0.065 in (1.651 mm) 0.109 in (2.769 mm) 0.140 in (3.556 mm) 0.191 in (4.851 mm) 1½ 40 1.900 in (48.26 mm) 0.065 in (1.651 mm) 0.109 in (2.769 mm) 0.145 in (3.683 mm) 0.200 in (5.080 mm) 2 50 2.375 in (60.33 mm) 0.065 in (1.651 mm) 0.109 in (2.769 mm) 0.154 in (3.912 mm) 0.218 in (5.537 mm) 2½ 65 2.875 in 0.083 in 0.120 in 0.203 in 0.276 in
prevalence varies depending on industry and geographical area. The pipe size designation generally includes two numbers; one that indicates the outside (OD) or nominal diameter, and the other that indicates the wall thickness. In the early twentieth century, American pipe was sized by inside diameter. This practice was abandoned to improve compatibility with pipe fittings that must usually fit the OD of the pipe, but it has had a lasting impact on modern standards around the world.
4.5 Sizes for Copper Tube
Copper tubing was introduced in about 1900, but didn't become popular until approximately 1950, depending on local building code adoption. Copper plumbing tube for residential plumbing follows an entirely different size system, often called Copper Tube Size (CTS); see table below. It’s nominal size is neither the inside nor outside diameter. Plastic tubing, such as PVC and CPVC, for plumbing applications also has different sizing standards. Common wall-thicknesses of copper tubing are "Type K", "Type L" and "Type M"
Type K has the thickest wall section of the three types of pressure rated
tubing and is commonly used for deep underground burial such as under sidewalks and streets, with a suitable corrosion protection coating or continuous polyethylene sleeve as required by code.
Type L has a thinner pipe wall section, and is used in residential and
commercial water supply and pressure applications.
Type M has the thinnest wall section, and is generally suitable for
condensate and other drains, but sometimes illegal for pressure applications, depending on local codes.
Outside diameter (OD)
Inside diameter (ID) (inches) Type K Type L Type M 3/8 1/2 0.402 0.43 0.45 1/2 5/8 0.528 0.545 0.569 5/8 3/4 0.652 0.668 0.69 3/4 7/8 0.745 0.785 0.811 1 1 1/8 0.995 1.025 1.055 1 1/4 1 3/8 1.245 1.265 1.291 1 1/2 1 5/8 1.481 1.505 1.527 2 2 1/8 1.959 1.985 2.009 2 1/2 2 5/8 2.435 2.465 2.495 3 3 1/8 2.907 2.945 2.981
Sizes for copper tubes
Types K and L are generally available in both hard drawn "sticks" and in rolls of soft annealed tubing, whereas type M is usually only available in hard drawn "sticks". Thin-walled types used to be relatively inexpensive, but since 2002 copper prices have risen considerably due to rising global demand and a
In the plumbing trade the size of copper tubing is measured by its nominal diameter (average inside diameter). Some trades, heating and cooling technicians for instance, use the outside diameter (OD) to designate copper tube sizes. The HVAC tradesman also use this different measurement to try and not confuse water pipe with copper pipe used for the HVAC trade, as pipe used in the Air-conditioning trade uses copper pipe that is made at the factory without processing oils that would be incompatible with the oils used to lubricate the compressors in the AC system. The OD of copper tube is always 1/8th inch larger than its nominal size. Therefore, 1" nominal copper tube and 1-1/8th" ACR tube are exactly the same tube with different size designations. The wall thickness of the tube, as mentioned above, never affects the sizing of the tube. Type K 1/2" nominal tube, is the same size as Type L 1/2" nominal tube (5/8" ACR).
4.6 Sizes for Stainless Steel Tube
Stainless steel pipes, which were coming into more common use in the mid 20th century, permitted the use of thinner pipe walls with much less risk of failure due to corrosion. This led to the development of stainless steel tubing, which due to it’s thinner wall it could not be threaded together according to
the ASME code, and therefore was fusion welded.
This led to the development of a range of hygienic stainless steel tube and fittings which could be used in applications requiring a clean and sanitary flow of liquids and where it is essential to avoid contamination of the products being carried. These applications cover the food processing, beverage, biotech and pharmaceutical industries including breweries and dairies.
The applications are low pressure with a maximum of 10 Bar. The products are available in grades 304L and-316L.
The size range is from ½”to 6 inch O/D.
The tube and fittings are of welded construction with the internal bead rolled and polished to eliminate crevices, thus preventing interruptions to the flow and eliminating the risk of contamination or bug traps as well as facilitate easy cleaning.
Hygienic tube and fittings are manufactured to the following standards including:
ASME BPE for pharmaceutical tube applications DIN 11850
O/D Wall Weight In swg mm kg/m 3/4 16 1.63 0.70 1 16 1.63 0.99 11/2 16 1.63 1.51 2 16 1.63 1.88 21/2 16 1.63 2.49 3 16 1.63 3.01 4 16 1.63 4.03 4 14 2.03 4.98 Sizes and weights for DN11850 Tube
O/D Wall Weight in mm kg/m 1 1.5 0.90 11/2 1.5 1.38 2 1.5 1.85 21/2 1.5 2.34 3 1.5 2.81 4 2.0 5.02
5.0 Pressure Ratings for Pipes and
5.1 Pressure Ratings for Pipe and Tube
The manufacture and installation of pressure piping is tightly regulated by the ASME "B31" code series such as B31.1 or B31.3 which have their basis in the ASME Boiler and Pressure Vessel Code. This code has the force of law in Canada and the USA. Europe has an equivalent system of codes. Pressure piping is generally classified as pipe that must carry pressures greater than 10 to 25 atmospheres, although definitions vary. To ensure safe operation of the system, the manufacture, storage, welding, testing, etc. of pressure piping must meet stringent quality standards.
In Europe, pressure piping uses the same pipe IDs and wall thicknesses as Nominal Pipe Size, but labels them with a metric Diameter Nominal (DN) instead of the imperial NPS. For NPS larger than 14, the DN is equal to the NPS multiplied by 25. (Not 25.4) This is documented by EN 10255 (formerly DIN 2448 and BS 1387) and ISO 65, and it is often called DIN or ISO pipe. In North America and the UK, pressure piping is usually specified by Nominal Pipe Size (NPS) and schedule (SCH). Pipe sizes are documented by a number of standards, including API 5L, ANSI/ASME B36.10M in the US, and BS 1600 and BS 1387 in the United Kingdom. Typically the pipe wall thickness is the controlled variable, and the Inside Diameter (I.D.) is allowed to vary. The pipe wall thickness has a variance of approximately 12.5 percent.
Key Learning Points
Identify why pipe and tube is classified as pressure rated Identify how to calculate the wall thickness required for a set
5.2 Wall Thickness Calculations for Straight
Pipe Under Internal Pressure
The following equations and tables are based on those provided in the Process Piping Specification, ASME B31.3a-2008, ASME Code for Pressure Piping. There are four equations which may be used to calculate the ‘pressure design wall thickness’ (t) of a straight pipe subject to internal pressure, two of which
are given as follows:
t = Pressure design thickness
d = Inside diameter of pipe. For pressure design calculation, the inside
diameter of the pipe is the maximum value allowable under the purchase specification.
P = Internal design pressure.
D = Outside diameter pipe as listed in tables of standards or
specifications or as measured.
Y = Coefficient from “Values of coefficient ‘Y’ for t<D/6” given in
the table below.
S = Stress value for material “Basic allowable stresses ‘S’ in tension for
stainless steels” given in the table below.
E = Quality factor, taken from the table below, “Basic quality factors
‘E’ for longitudinal weld joints in stainless steel pipes, tubes and fittings”.
The equations assume t<D/6 (for pipe with t >D/6 or P/SE >0.385
additional factors need to be considered).
Materials Temperature, °F (°C) ≤900 ( ≤482) 950 (510) 1000 (538) 1050 (566) 1100 (593) ≥1150 ( ≥621) Y Ferritic Steels 0.4 0.5 0.7 0.7 0.7 0.7 Austenitic Steels 0.4 0.4 0.4 0.4 0.5 0.7 Cast Iron 0.0 - - - -
ASTM Spec No. Grade Min Temp °F (for °C see Notes) Metal Temperature, °F (°C) Notes Min Temp to 100 (37.8) 300 (149) 500 (260) 700 (371) 850 (454) 1000 (538) 1150 (621) 1300 (704) 1400 (760) 1500 (816)
Basic Allowable Stress, S ksi
A312 TP321 -325 16.7 16.7 16.1 14.6 14.0 13.5 5.0 1.7 0.8 0.3 1, 2 A376 TP321 -325 16.7 16.7 16.1 14.6 14.0 13.5 5.0 1.7 0.8 0.3 1, 2 A269 TP304L -425 16.7 16.7 14.8 13.5 12.8 7.8 4.0 2.1 1.1 0.9 2, 3 A312 TP304L -425 16.7 16.7 14.8 13.5 12.8 7.8 4.0 2.1 1.1 0.9 - A358 304L -425 16.7 16.7 14.8 13.5 12.8 7.8 4.0 2.1 1.1 0.9 2 A269 TP316L -325 16.7 16.7 14.4 12.9 12.1 11.2 8.8 3.5 1.8 1.0 2, 3 A312 TP316L -325 16.7 16.7 14.4 12.9 12.1 11.2 8.8 3.5 1.8 1.0 - A358 316L -325 16.7 16.7 14.4 12.9 12.1 11.2 8.8 3.5 1.8 1.0 2 A312 TP321 -325 16.7 16.7 16.1 14.6 14.0 13.5 6.9 3.2 1.9 1.1 1, 2, 4 A376 TP321 -325 16.7 16.7 16.1 14.6 14.0 13.5 6.9 3.2 1.9 1.1 1, 2, 4 A312 TP321H -325 16.7 16.7 16.1 14.6 14.0 13.5 6.9 3.2 1.9 1.1 1, 2 A376 TP321H -325 16.7 16.7 16.1 14.6 14.0 13.5 6.9 3.2 1.9 1.1 - A268 TP409 -20 20.0 - - - 6 A268 TP430Ti -20 20.0 - - - 6, 7 A376 16-8-2H -325 20.0 - - - 5, 6,8 A268 TP405 -20 20.0 17.7 17.2 16.2 10.4 4.0 - - - - 6 A268 TP410 -20 20.0 17.7 17.2 16.2 10.4 6.4 1.8 - - - 6 A268 TP430 -20 20.0 19.6 19.0 17.6 10.4 6.5 2.4 - - - 6, 7 A312 TP317L -325 20.0 20.0 17.7 16.2 15.2 - - - - A312 TP310 -325 20.0 20.0 20.0 18.3 14.6 11.0 3.6 0.8 0.4 0.2 4, 6, 10 A358 310S -325 20.0 20.0 20.0 18.3 14.6 11.0 3.6 0.8 0.4 0.2 2, 4, 5, 6 A409 TP310 -325 20.0 20.0 20.0 18.3 14.6 11.0 3.6 0.8 0.4 0.2 2, 4, 5,6, 10 A312 TP321 -325 20.0 20.0 19.3 17.5 16.7 16.2 5.0 1.7 0.8 0.3 1 A358 321 -325 20.0 20.0 19.3 17.5 16.7 16.2 5.0 1.7 0.8 0.3 1, 2 A376 TP321 -325 20.0 20.0 19.3 17.5 16.7 16.2 5.0 1.7 0.8 0.3 1, 2 A409 TP321 -325 20.0 20.0 19.3 17.5 16.7 16.2 5.0 1.7 0.8 0.3 1, 2 A312 TP309 -325 20.0 20.0 20.0 18.3 14.6 10.5 5.0 2.3 1.3 0.7 4, 6, 10 A358 309S -325 20.0 20.0 20.0 18.3 14.6 10.5 5.0 2.3 1.3 0.7 4, 5, 6, 2 A409 TP309 -325 20.0 20.0 20.0 18.3 14.6 10.5 5.0 2.3 1.3 0.7 2, 4, 5, 6, 10 A312 TP347 -425 20.0 20.0 19.9 18.6 18.2 18.0 6.1 2.2 1.2 0.8 - A358 347 -425 20.0 20.0 19.9 18.6 18.2 18.0 6.1 2.2 1.2 0.8 1, 2 A376 TP347 -425 20.0 20.0 19.9 18.6 18.2 18.0 6.1 2.2 1.2 0.8 1, 2 A409 TP347 -425 20.0 20.0 19.9 18.6 18.2 18.0 6.1 2.2 1.2 0.8 1, 2 A312 TP348 -325 20.0 20.0 19.9 18.6 18.2 18.0 6.1 2.2 1.2 0.8 - A358 348 -325 20.0 20.0 19.9 18.6 18.2 18.0 6.1 2.2 1.2 0.8 1, 2 A376 TP348 -325 20.0 20.0 19.9 18.6 18.2 18.0 6.1 2.2 1.2 0.8 1, 2 A409 TP348 -325 20.0 20.0 19.9 18.6 18.2 18.0 6.1 2.2 1.2 0.8 1, 2 A312 TP310 -325 20.0 20.0 20.0 18.3 14.6 11.0 7.3 3.5 1.6 0.8 4, 6, 10, 11
A269 TP316 -425 20.0 20.0 17.9 16.3 15.7 15.3 9.8 4.1 2.3 1.3 5, 8 A312 TP316 -425 20.0 20.0 17.9 16.3 15.7 15.3 9.8 4.1 2.3 1.3 4, 8 A358 316 -425 20.0 20.0 17.9 16.3 15.7 15.3 9.8 4.1 2.3 1.3 2, 4, 5, 8 A376 TP316 -425 20.0 20.0 17.9 16.3 15.7 15.3 9.8 4.1 2.3 1.3 2, 4, 5, 8 A409 TP316 -425 20.0 20.0 17.9 16.3 15.7 15.3 9.8 4.1 2.3 1.3 2, 4, 5,8 A312 TP317 -325 20.0 20.0 17.9 16.3 15.7 15.3 9.8 4.1 2.3 1.3 4, 8 A409 TP317 -325 20.0 20.0 17.9 16.3 15.7 15.3 9.8 4.1 2.3 1.3 2, 4, 5, 8
Spec No. Class (or Type) Description E Notes A182 - Forgings and Fittings 1.00
- Seamless Tube 1.00 -- Electric Fusion Welded Tube, Double Butt Seam 0.85 -- Electric Fusion Welded Tube, Single Butt Seam 0.80
- Seamless Tube 1.00 -- Electric Fusion Welded Tube, Double Butt Seam 0.85 -- Electric Fusion Welded Tube, Single Butt Seam 0.80
- Seamless Pipe 1.00 -- Electric Fusion Welded Pipe, Double Butt Seam 0.85 -- Electric Fusion Welded Pipe, Single Butt Seam 0.80
1, 3, 4 Electric Fusion Welded Pipe, 100% radiographed 1.00 -5 Electric Fusion Welded Pipe, Spot radiographed 0.90 -2 Electric Fusion Welded Pipe, Double Butt Seam 0.85 - A376 - Seamless Pipe 1.00
- Seamless Fittings 1.00 -- Welded Fitting, 100% radiographed 1.00 1 - Welded Fitting, Double Butt Seam 0.85 -- Welded Fitting, Single Butt Seam 0.80
- Electric Fusion Welded Pipe, Double Butt Seam 0.85 -- Electric Fusion Welded Pipe, Single Butt Seam 0.80 - A430 - Seamless Pipe 1.00
- Seamless 1.00
-- Electric Fusion Welded Pipe, 100% radiographed 1.00 -- Electric Fusion Welded Tube, Double Butt Seam 0.85
-6.0 Physical Properties of Piping
6.1 Physical Properties of Piping Materials
The reasons pipe and tube are made from different materials is due the to physical properties of different materials. Properties such as:
Malleability Ductility Brittleness Hardness Elasticity Conductivity
Chemical resistance / resistance to corrosion
Malleability can be defined as the property of a metal to be deformed by compression without cracking or rupturing. This property is very useful for copper tubing systems which allows the tube to be bent to follow the required route quickly without the need for expensive and time consuming fittings:
Ductility is a mechanical property used to describe the extent to which materials can be deformed plastically without fracture. Ductile metals lend themselves to be formed into desired cross sectional shapes easier and therefore are cheaper to manufacture
The tendency for a metal to crack or break with deformation. Metals displaying this property are not readily used for pipe or tube as this is a disadvantage to a material.
Is the property of being rigid and resistant to pressure; not easily scratched. It is measured on Mohs scale. It’s presence in metals can be an advantage for high pressure systems but can be a disadvantage as it can increase machining, cutting and fabrication times.
Key Learning Points
Identify different physical properties of piping materials Define the physical properties
Identify how these properties can effect the choice of pipe for
The property by virtue of which a material deformed under the load can regain its original dimensions when unloaded. This property is utilized in piping system designs where pipes may expand or contract due to temperature differences. The elasticity of piping materials can help the designer cater for this.
The ability of a material to conduct electrical current or heat. Some piping systems high conductivity metals for high heat transfer while other piping systems use low conductivity plastic materials to prevent heat transfer.
Chemical resistance/ Resistance to Corrosion
The degree to which a material resists the corrosive action of industrial chemicals. This is probably the most significant property which affects the choice of piping material and is the biggest contributor to the price of material. Specialist alloys of stainless steel such as Hastelloy can be 10 to 20 times more expensive that standard stainless steel and can be slower to fit and weld which increase installation costs.
Nayyar, P.E., Mohinder L. (2000). "A1". in Mohinder L. Nayyar, P.E..
Piping Handbook(7th ed.). New York: McGraw-Hill. ISBN 0-07-047106-1.
David L. Goetsch (2000).
Technical Drawing(5th ed.). Thompson
Delmar Learning ISBN: 1-4018-5760-4
International standard ISO 7-1: Pipe threads where pressure-tight joints
are made on the threads — Part 1: Dimensions, tolerances and
designation. International Organization for Standardization, Geneva.
BS EN 10226: Pipe threads where pressure tight joints are made on the
threads. (The European version of ISO 7.)
Part 1: Taper external threads and parallel internal threads —
Dimensions, tolerances and designation.
Part 2: Taper external threads and taper internal threads —
Dimensions, tolerances and designation.
BS 21: Pipe threads for tubes and fittings where pressure-tight joints
are made on the threads (metric dimensions). British Standards Institution, 1985. (Superseded by BS EN 10226:2004).
International standard ISO 228-1: Pipe threads where pressure-tight
joints are not made on the threads — Part 1: Dimensions, tolerances and designation.
BS 2779: Specification for pipe threads for tubes and fittings where
pressure-tight joints are not made on the threads (metric dimensions), 1986.
BS EN 10226-1:2004
ASME B31.9 Building Services Piping; 937 – Leak Testing, 1996 Edition Elements of Plumbing by Samuel Edward Dibble, 2010